Activation of Carbon Porous Paper for Alkaline Alcoholic Fuel Cells

: In this study, various treatment methods to increase the reactivity of carbon porous electrodes for alkaline alcoholic fuel cells were investigated with commercially available carbon papers to understand the characteristic electrochemical behaviors of the treated carbon electrodes and to ﬁnd the best method to enhance the cell performance. E ﬀ ects of thermal treatment, potassium hydroxide (KOH) treatment, N 2 doping, and reaction-area control via a multi-layered structure were compared in the cell-based tests, and a huge improvement in the cell performance (i.e., 64% increase of open circuit voltage (OCV) and 320% increase of max power density) was found from the thermal-treated four-layered carbon porous electrode. The results were compared with those from platinum on carbon (Pt / C)-based cells, and a discussion on the direction of research in the future was conducted. The results of this study are expected to provide key guidelines for alcoholic fuel cell (AFC) developers to develop cost-e ﬀ ective AFC with a carbon electrode.


Introduction
A fuel cell is a system employed to convert the chemical energy of fuels into electrical energy without generating any emission gasses, and it is thus considered one of the most promising power sources to replace the conventional fossil fuel-based systems in order to preserve a clean and sustainable environment. In particular, alcoholic fuel cells (AFC) using easy-to-carry liquid alcoholic fuel have been considered to replace conventional batteries, especially for portable electronic devices, due to their benefits of continuous electricity generation without the need of long-time charge and the light weight of the system [1]. Intensive research on AFC has been conducted, but it has not been able to reach a full commercialization state due to the challenging issues of catalyst poisoning and reactant crossover [2][3][4].
Recently, a new AFC system based on alkaline chemistry was reported as one of the most promising systems to resolve the challenging issues of the conventional acid-type AFC [1,2,5,6]. The kinetics of electro-chemical reactions in alkaline medium is known to be very fast, which allows inexpensive but CO-tolerable materials to be used as an electrode, resolving the catalyst poisoning issue of the conventional system. In particular, the charge carrier OH − moves through the ion-exchange membrane from the cathode to anode side (i.e., opposite to the direction of the conventional acid-based AFC) of the cell during operation, and thereby prevents the alcohol crossover and flooding issue on the cathode side, which is one of the key issues of the conventional acid AFC system [1].
A high reactivity, one of the excellent benefits in alkaline AFC, has driven research to replace the expensive Pt-based catalyst needed for an oxygen reduction reaction (ORR) with inexpensive Energies 2019, 12, 3207 3 of 12 of a system of interest. In this study, four activation methods available in the literature, such as thermal treatment, the N 2 doping method, chemical treatment with KOH, and reaction-area control via a multi-layered structure, will be utilized to activate the conventional carbon papers which are commercially available. First of all, the best conditions for each treatment method will be defined through cell-based performance tests. Then, the defined conditions will be applied to prepare the carbon electrode samples, and cell tests with those samples will be conducted. The results will be compared with the target performance defined from a cell with a Pt/C-coated electrode. The results of this study are expected to provide key guidelines for AFC cell developers so that they are able to develop cost-effective AFC with a carbon electrode.

Treatment of the Membrane
The KOH-treated cation-exchange membrane (N212, Ion Power) was utilized for this study due to the easy access to the membrane material. The membrane was treated by immersing small pieces of it 3 in × 3 in in boiling de-ionized (DI) water for 1 h and then 6 M KOH (Sigma Aldrich, PO Box 14508 St. Louis, MO 63178 USA) solution at 80 • C for 1 h. The treated membrane was rinsed several times with DI water to remove extra alkaline solution.
When KOH solution is added to the methanol fuel reservoir, hydroxyl anions (OH − ) are formed in the anode fuel solution: Then, the methanol reacts electrochemically with the hydroxide ions at the reaction sites on the anode electrode to produce water and electrons: The generated electrons in the anode, as shown in Equation (2), pass through an external electrical circuit to reach the cathode side to take part in the electrochemical reaction with externally provided oxygen and water at the cathode electrode to generate hydroxyl anions, as illustrated in Equation (3). The negative charges of the hydroxyl anions are balanced by K + coming from the anode side to satisfy the electro-neutral state. Therefore, K + is a spectator ion which does not take an active part in the reaction, and also does not carry water or methanol, preventing cathode-flooding or methanol cross-over issues. The overall reaction is described in Equation (4), and the cell voltage of 1.21 V can be obtained theoretically for a standard condition.
The overall reaction is

Preparation of the Pt/C-Coated Carbon Porous Electrode
The methanol reaction in the anode side needs a catalyst to enhance the electrochemical reaction, and a Pt-based catalyst has been utilized for most of the AFC. In this study, a Pt/C-coated carbon porous electrode (CPE) was used, and it was prepared by the following method: a proper amount of (10% Pt/C) platinum powder was measured so that 0.5 mg of Pt was coated for every 1 cm 2 area of carbon paper (i.e., Sigracet 10 BC, Ion Power). The Pt/C powder was placed in a vial, and 1 µL of DI water was added for every 1 mg of platinum powder. A total of 6.67 µL of Nafion solution and Energies 2019, 12, 3207 4 of 12 5.33 µL of pure iso-propanol were added for every 1 mg of platinum powder and the mixture was stirred by a magnetic stirrer for about 20 min to form a slurry or thick solution. The slurry was painted on the microporous layer (MPL) side of the carbon paper by a paintbrush, and was then dried at room temperature for about 24 h [30]. The prepared Pt/C-coated CPE was used as an electrode for the anode side for all the tests conducted in this study, and it was applied to both the anode and cathode sides for the test to set up the target cell performance.

Thermal Treatment to Activate the Carbon Porous Electrode
In order to activate the CPE via thermal treatment, 1 in × 1 in pieces of the carbon paper (Sigracet 10 AA, Ion Power) were placed in a furnace which was open to the air environment, and were heated at 300 • C, 400 • C, and 500 • C for 10 h and 20 h [12]. The treated samples were washed several times with diluted isopropyl alcohol to remove dusts or debris left inside.

Chemical Treatment to Activate the Carbon Porous Electrode
Pieces (1 in × 1 in) of carbon paper were submerged in 20% aqueous KOH solution at room temperature overnight, and were dried in an oven. Then, the samples were positioned in an argon quartz tube furnace (GSL-1100X, MTI, 860 S. 19th Street, Richmond, CA 94804-3809, USA), and thermally heated at temperatures from 500 • C to 800 • C for 40 min, minimizing possible effects by oxidizing impure gases [28]. Additionally, the treated samples were washed several times with diluted isopropyl alcohol, and dried before using them for the cell test.

Nitrogen Doping to Activate the Carbon Porous Electrode
The incorporation of nitrogen moieties into the carbon structure was conducted by pyrolyzing melamine (C 3 H 6 N 6 ) (Sigma Aldrich), which has three triazine heterocyclic organic compounds, as a nitrogen-contained precursor. Pieces of carbon paper (1 in × 1 in) were washed several times by dilute acetone, and were then soaked in the aqueous melamine solution overnight to absorb enough melamine inside. They were dried in an oven, and were positioned in the argon quartz tube furnace (GSL-1100X, MTI) at 900 • C for 10, 20, and 30 h [27]. At this high temperature, the melamine absorbed in the porous carbon paper was split to release free nitrogen, which dopes at surfaces of carbon material.

Cell Structure and Test
A unit cell consists of a KOH-treated membrane in the middle, Pt/C-coated CPE and serpentine flow field on the anode side, and activated CPE and the serpentine flow field on the cathode side. The cell was assembled by compressing cell components stacked in the sequence (i.e., Anode flowfield|Pt/C-coated CPE|membrane|activated CPE|cathode flow field) by eight bolts to minimize the electrical contact resistance among the components.

Baseline Performance of the Carbon Electrode and Pt/C-Coated Electrode
A cell performance test was conducted first, with a cell having untreated CPE as a cathode electrode, in order to have a baseline performance for carbon electrode material. Additionally, a cell with Pt/C CPE on the cathode side was tested to setup the target performance to achieve with the carbon electrode. Both the cell tests were conducted with the same operating conditions and cell structure, except for the cathode-electrode material, and the difference in the measured performance was thus the direct result of reactivity difference in the utilized electrode materials.
As shown in Figure 2, the performance of the cell with untreated CPE was significantly lower than that of the cell with Pt/C, as expected. The open circuit voltage (OCV) was around 0.5 V, which is 44% less than that of the Pt/C-cell, and the maximum current density was around 10 mA/cm 2 , which is 61% less than the Pt/C-cell, indicating that the carbon paper cannot be used in the AFC unless it is activated. Various methods will be applied in this study to activate carbon paper to increase the cell performance, and all the details of these treatments and results will be described in the subsequent sections.

Baseline Performance of the Carbon Electrode and Pt/C-Coated Electrode
A cell performance test was conducted first, with a cell having untreated CPE as a cathode electrode, in order to have a baseline performance for carbon electrode material. Additionally, a cell with Pt/C CPE on the cathode side was tested to setup the target performance to achieve with the carbon electrode. Both the cell tests were conducted with the same operating conditions and cell structure, except for the cathode-electrode material, and the difference in the measured performance was thus the direct result of reactivity difference in the utilized electrode materials.
As shown in Figure 2, the performance of the cell with untreated CPE was significantly lower than that of the cell with Pt/C, as expected. The open circuit voltage (OCV) was around 0.5 V, which is 44% less than that of the Pt/C-cell, and the maximum current density was around 10 mA/cm 2 , which is 61% less than the Pt/C-cell, indicating that the carbon paper cannot be used in the AFC unless it is activated. Various methods will be applied in this study to activate carbon paper to increase the cell performance, and all the details of these treatments and results will be described in the subsequent sections.

Baseline Performance of the Carbon Electrode and Pt/C-Coated Electrode
A cell performance test was conducted first, with a cell having untreated CPE as a cathode electrode, in order to have a baseline performance for carbon electrode material. Additionally, a cell with Pt/C CPE on the cathode side was tested to setup the target performance to achieve with the carbon electrode. Both the cell tests were conducted with the same operating conditions and cell structure, except for the cathode-electrode material, and the difference in the measured performance was thus the direct result of reactivity difference in the utilized electrode materials.
As shown in Figure 2, the performance of the cell with untreated CPE was significantly lower than that of the cell with Pt/C, as expected. The open circuit voltage (OCV) was around 0.5 V, which is 44% less than that of the Pt/C-cell, and the maximum current density was around 10 mA/cm 2 , which is 61% less than the Pt/C-cell, indicating that the carbon paper cannot be used in the AFC unless it is activated. Various methods will be applied in this study to activate carbon paper to increase the cell performance, and all the details of these treatments and results will be described in the subsequent sections.  It should be noted that the performance measured in this study may be different from what is reported in the literature due to the difference in cell components, and we will thus utilize the cell polarization behaviors plotted with respect to the current density normalized by the maximum current density to compare the relative performance for various activation methods on the same scale.

Thermal Treatment (Thermal Oxidation)
The effect of thermal treatment (or thermal oxidation) was analyzed by comparing the performances of cells consisting of the cathode CPEs, which were treated at 300 • C, 400 • C, and 500 • C for 10 h and 20 h in the air environment. For the anode side, the Pt/C-coated electrode was applied for all cell tests. The polarization behaviors were measured with respect to the current density normalized by the maximum current density to compare the relative performance clearly, as described previously.
As shown in Figure 3, especially for the cases of CPEs thermally treated at 300 • C, 400 • C, and 500 • C for 10 h, voltages at a zero current (i.e., open circuit voltage, OCV) were not so different for all the treated samples, but in the kinetic limited zone (i.e., performance at a low current density), a significant voltage drop was found from all samples except the CPE, which was treated at 500 • C for 10 h, indicating that the kinetic property for this sample was improved. Additionally, the ohmic property, which can be estimated by the slope of voltage drop vs. current in the linear region of the plot, was not so different for all the samples. However, the big difference in performance was found in the high current region, which is known as the mass transfer limited region, and the performance was improved as the treatment temperature increased, indicating that the treatment temperature directly affected the mass transfer property. current density to compare the relative performance for various activation methods on the same scale.

Thermal Treatment (Thermal Oxidation)
The effect of thermal treatment (or thermal oxidation) was analyzed by comparing the performances of cells consisting of the cathode CPEs, which were treated at 300 °C, 400 °C, and 500 °C for 10 h and 20 h in the air environment. For the anode side, the Pt/C-coated electrode was applied for all cell tests. The polarization behaviors were measured with respect to the current density normalized by the maximum current density to compare the relative performance clearly, as described previously.
As shown in Figure 3, especially for the cases of CPEs thermally treated at 300 °C, 400 °C, and 500 °C for 10 h, voltages at a zero current (i.e., open circuit voltage, OCV) were not so different for all the treated samples, but in the kinetic limited zone (i.e., performance at a low current density), a significant voltage drop was found from all samples except the CPE, which was treated at 500 °C for 10 h, indicating that the kinetic property for this sample was improved. Additionally, the ohmic property, which can be estimated by the slope of voltage drop vs. current in the linear region of the plot, was not so different for all the samples. However, the big difference in performance was found in the high current region, which is known as the mass transfer limited region, and the performance was improved as the treatment temperature increased, indicating that the treatment temperature directly affected the mass transfer property.
These results (i.e., improvement of kinetic and mass transfer properties) can be understood from the effect induced by thermal treatment in the air environment. The oxygen species introduced into the carbon matrix during the treatment facilitate the electrochemical reaction by increasing kinetics [12], and they also render the surface hydrophilic, allowing the aqueous-based reactants to readily access the porous electrode, and thereby mass transfer could be enhanced [14][15][16]. However, when the treatment time was increased further to 20 h, the cell performance dropped significantly, which is due to degradation of the carbon matrix caused by excessive oxidation during the treatment. This conclusion is supported by the dimension change (10%-20% thickness change) of the carbon paper treated at 500 °C for 20 h.  These results (i.e., improvement of kinetic and mass transfer properties) can be understood from the effect induced by thermal treatment in the air environment. The oxygen species introduced into the carbon matrix during the treatment facilitate the electrochemical reaction by increasing kinetics [12], and they also render the surface hydrophilic, allowing the aqueous-based reactants to readily access the porous electrode, and thereby mass transfer could be enhanced [14][15][16]. However, when the treatment time was increased further to 20 h, the cell performance dropped significantly, which is due to degradation of the carbon matrix caused by excessive oxidation during the treatment. This conclusion is supported by the dimension change (10%-20% thickness change) of the carbon paper treated at 500 • C for 20 h.

Chemical Treatment (KOH-Heat Treatment)
Four treated CPEs (i.e., at 500 • C, 600 • C, 700 • C, and 800 • C for 40 min in an argon environment after KOH treatment) were prepared as described in the experimental section, and the performance was measured from the cells with treated CPEs. As shown in Figure 4, for the case of 600 • C, 700 • C, and 800 • C treated CPEs, the behaviors of kinetic loss (drop in cell voltage in a low current range), ohmic loss (slope of voltage drop vs. current), and mass transfer loss (voltage drop in a high current range) are very similar in all three cases, and their graph lines are shifted on the y-axis by several voltages (0.3 to 0.5 V) from each other.

Chemical Treatment (KOH-Heat Treatment)
Four treated CPEs (i.e., at 500 °C, 600 °C, 700 °C, and 800 °C for 40 min in an argon environment after KOH treatment) were prepared as described in the experimental section, and the performance was measured from the cells with treated CPEs. As shown in Figure 4, for the case of 600 °C, 700 °C, and 800 °C treated CPEs, the behaviors of kinetic loss (drop in cell voltage in a low current range), ohmic loss (slope of voltage drop vs. current), and mass transfer loss (voltage drop in a high current range) are very similar in all three cases, and their graph lines are shifted on the y-axis by several voltages (0.3 to 0.5 V) from each other. This behavior is very similar to the case of reaction-area control via a multi-layered structure, as explained in the last section of the treatment effect, and it can thus be concluded that KOH treatment mostly increases the reaction area without further changing other properties, such as kinetics, ohmic, and mass transfer in the treatment temperature range from 600 °C to 800 °C. This conclusion is supported by the literature [28,31,32], which reports that KOH activation improves the specific surface area of carbon, resulting in a significant increase of capacity for the super-capacitor application. This characteristic behavior can be further understood by considering the activation conditions when the samples were heated in an inert Ar gas environment. Therefore, the effect of oxidizing impure gases, which are known to significantly change the properties of carbon material, could be eliminated, resulting in no sensible change of other properties. It is a very interesting result, and detailed study to define the reason for this behavior is required, which represents future work. For the case of 500 °C treatment, a very low performance was found, indicating that the treatment temperature was not high enough to activate the carbon material.

Nitrogen Doping
Nitrogen was doped on the surface of carbon porous papers at 900 °C for 10 h, 20 h, and 30 h in an argon environment. Its effect on the cell performance was compared with the polarization curve, as shown in Figure 5. As the treatment time increased from 10 h to 20 h, the overall voltage was decreased slightly by 30 mV, and as the treatment time increased further to 30 h, a significant performance drop by 90 mV was found, indicating that the carbon matrix in the carbon paper may have been degraded during the extended exposure to a high temperature.
It should be noted that this high temperature is a general condition in doping nitrogen to carbon This behavior is very similar to the case of reaction-area control via a multi-layered structure, as explained in the last section of the treatment effect, and it can thus be concluded that KOH treatment mostly increases the reaction area without further changing other properties, such as kinetics, ohmic, and mass transfer in the treatment temperature range from 600 • C to 800 • C. This conclusion is supported by the literature [28,31,32], which reports that KOH activation improves the specific surface area of carbon, resulting in a significant increase of capacity for the super-capacitor application. This characteristic behavior can be further understood by considering the activation conditions when the samples were heated in an inert Ar gas environment. Therefore, the effect of oxidizing impure gases, which are known to significantly change the properties of carbon material, could be eliminated, resulting in no sensible change of other properties. It is a very interesting result, and detailed study to define the reason for this behavior is required, which represents future work. For the case of 500 • C treatment, a very low performance was found, indicating that the treatment temperature was not high enough to activate the carbon material.

Nitrogen Doping
Nitrogen was doped on the surface of carbon porous papers at 900 • C for 10 h, 20 h, and 30 h in an argon environment. Its effect on the cell performance was compared with the polarization curve, as shown in Figure 5. As the treatment time increased from 10 h to 20 h, the overall voltage was decreased slightly by 30 mV, and as the treatment time increased further to 30 h, a significant performance drop by 90 mV was found, indicating that the carbon matrix in the carbon paper may have been degraded during the extended exposure to a high temperature. impregnated in their manufacturing process [33], and thus, those additives holding the matrix structure of carbon fibers together may have been degraded in this harsh condition of long exposure to a high-temperature environment, leading to a significant decrease of cell performance. This degradation of CPE can be understood by the dimensional change (10%-20% of thickness reduction) of carbon papers after the treatment at 900 °C for 30 h.

Figure 5.
Effect of nitrogen-doping of the carbon porous electrode (CPE) on the cell performance. The cell performance was decreased as the treatment time increased, which is due to degradation of the carbon matrix.

Reaction-Area Control via a Multi-Layered Structure
The inexpensive standard carbon paper which is commercially available was utilized to control the reaction area by stacking several sheets of papers on top of each other to make multi-layered paper electrodes (thickness of one layer is about 0.35 mm).
As illustrated in Figure 6, OCV was increased from 0.48 V for one layer to 0.64 V for four layers (i.e., 33% increase), but there were no big differences in the ohmic property found for the multilayered electrodes, which seems to contradict the research results in the flow battery area [13]. However, this behavior can be understood by checking the operating current ranges. The current condition of the AFC is several orders of magnitude smaller than that of the flow battery, and thus, the effect of the ohmic drop was not significant (i.e., = × ). In the case of three-and fourlayered electrodes, cells were able to be operated at higher current conditions than the cases of oneand two-layered electrodes. This behavior is due to the increased available reaction area in the multilayered electrodes, where reactants can access the reaction sites relatively easily, and thus the mass transfer property can be enhanced, which is consistent with the results for the flow battery [13,16]. It is possible to check the performance variation with more than four sheets of paper, but according to the literature [14,15,34], the use of more than four sheets showed a decrease in the performance, so we did not conduct the cell test with more than four sheets. It should be noted that this high temperature is a general condition in doping nitrogen to carbon [9,27], but in this experiment, we used carbon porous papers, which have resins and binders impregnated in their manufacturing process [33], and thus, those additives holding the matrix structure of carbon fibers together may have been degraded in this harsh condition of long exposure to a high-temperature environment, leading to a significant decrease of cell performance. This degradation of CPE can be understood by the dimensional change (10%-20% of thickness reduction) of carbon papers after the treatment at 900 • C for 30 h.

Reaction-Area Control via a Multi-Layered Structure
The inexpensive standard carbon paper which is commercially available was utilized to control the reaction area by stacking several sheets of papers on top of each other to make multi-layered paper electrodes (thickness of one layer is about 0.35 mm).
As illustrated in Figure 6, OCV was increased from 0.48 V for one layer to 0.64 V for four layers (i.e., 33% increase), but there were no big differences in the ohmic property found for the multi-layered electrodes, which seems to contradict the research results in the flow battery area [13]. However, this behavior can be understood by checking the operating current ranges. The current condition of the AFC is several orders of magnitude smaller than that of the flow battery, and thus, the effect of the ohmic drop was not significant (i.e., η ohm = I × R). In the case of three-and four-layered electrodes, cells were able to be operated at higher current conditions than the cases of one-and two-layered electrodes. This behavior is due to the increased available reaction area in the multi-layered electrodes, where reactants can access the reaction sites relatively easily, and thus the mass transfer property can be enhanced, which is consistent with the results for the flow battery [13,16]. It is possible to check the performance variation with more than four sheets of paper, but according to the literature [14,15,34], the use of more than four sheets showed a decrease in the performance, so we did not conduct the cell test with more than four sheets. The thickness of the electrode was controlled by stacking sheets of carbon paper to make the multi-layered structure.

Optimal Treatment Condition
So far, the effects of various treatment methods on the cell performance have been compared, and the best conditions for each treatment have been found. In particular, the multi-layered structure was found to be effective at increasing the performance, and thus, this method was applied to the cells with the samples treated via the best pretreatment conditions (i.e., N2-doped four-layered CPE, KOH-treated four-layered CPE, and thermal-treated four-layered CPE) to further increase the cell performance. The cell performances were compared with baseline (from untreated carbon paper) and target (from Pt/C CPE) performances, as illustrated in Figure 7 and Table 1, with key performance data points.  The thickness of the electrode was controlled by stacking sheets of carbon paper to make the multi-layered structure.

Optimal Treatment Condition
So far, the effects of various treatment methods on the cell performance have been compared, and the best conditions for each treatment have been found. In particular, the multi-layered structure was found to be effective at increasing the performance, and thus, this method was applied to the cells with the samples treated via the best pretreatment conditions (i.e., N 2 -doped four-layered CPE, KOH-treated four-layered CPE, and thermal-treated four-layered CPE) to further increase the cell performance. The cell performances were compared with baseline (from untreated carbon paper) and target (from Pt/C CPE) performances, as illustrated in Figure 7 and Table 1, with key performance data points.
Energies 2019, 12, x FOR PEER REVIEW 9 of 12 Figure 6. Effect of the thickness of the carbon porous electrode (CPE) on the cell performance. The thickness of the electrode was controlled by stacking sheets of carbon paper to make the multi-layered structure.

Optimal Treatment Condition
So far, the effects of various treatment methods on the cell performance have been compared, and the best conditions for each treatment have been found. In particular, the multi-layered structure was found to be effective at increasing the performance, and thus, this method was applied to the cells with the samples treated via the best pretreatment conditions (i.e., N2-doped four-layered CPE, KOH-treated four-layered CPE, and thermal-treated four-layered CPE) to further increase the cell performance. The cell performances were compared with baseline (from untreated carbon paper) and target (from Pt/C CPE) performances, as illustrated in Figure 7 and Table 1, with key performance data points.   In the case of OCV, the cell with untreated CPE produced 0.48 V (i.e., half of that of the Pt/C case), but it was improved to 0.725, 0.74, and 0.79 (64% increase) as CPE was treated with N 2 doping, KOH, and the thermal method, respectively. The performance gain was also compared with the maximum current density values. It was 10 mA/cm 2 for untreated CPE, but increased up to 22 mA/cm 2 (120% increase) by thermal treatment, which is just 4 mA/cm 2 less than that of Pt/C. The maximum power density was also compared, and it was 0.84 mW/cm 2 in the baseline, but increased to 3.6 mW/cm 2 (320% increase) with thermal treatment.
Even though the cell performance was significantly improved by combining the thermal treatment method and a multi-layered structure, the performance was still much lower than that of Pt/C. However, the price of Pt is several orders of magnitude higher than carbon, and therefore, the results of this research using inexpensive standard carbon paper are promising. Additionally, a further increase of OCV and kinetics is required, which may be achieved by applying carbon particles to the porous electrode to increase the reaction area, as shown in the literature [35].

Conclusions
In this study, alkaline alcoholic fuel cells (AFC) were investigated as a promising system to replace the conventional battery systems due to their benefits of continuous electricity generation without the need for long-time charge and the light weight of the system. The possibility of replacing the Pt-based electrode with a carbon porous electrode for an oxygen reduction reaction was studied with cell-based tests. Various methods, such as thermal treatment, KOH treatment, the N 2 doping method, and reaction-area control via a multi-layered structure, were utilized to increase the reactivity of the carbon electrode, and the characteristic electrochemical reactive behaviors of the carbon electrodes treated by each method were analyzed.
It was found that the activation and mass transfer properties were significantly enhanced through the thermal treatment method, whereas a simple voltage shift without a sensible change of other properties was found from the treatment of KOH and the multi-layered electrode. Harsh treatment conditions, such as thermal treatment (i.e., thermal oxidation) at 500 • C for longer than 20 h and N 2 doping at 900 • C for longer than 20 h, were found to degrade the carbon porous electrode significantly, resulting in a substantial drop in the cell performance. Therefore, those conditions should be avoided. A significant improvement in the cell performance was achieved (2.3 times increase of max power density) by commercially available carbon papers prepared with methods defined in this study, providing a new direction of research in which conventional carbon papers are used as a promising electrode for alkaline AFC. However, the performance was still much lower than that of Pt/C, and a further increase of the cell performance is required to replace the Pt/C-electrode, which represents the future work.